Study on the Constitutive Relationship between Ordinary Concrete and Nano-Titanium Dioxide-Modified Concrete at High Temperature

After high-temperature treatment, both nano-titanium dioxide-modified concrete and ordinary concrete exhibit typical splitting failure. High-temperature heating reduces the mechanical properties and brittleness of concrete and improves the ductility of concrete. The stress–strain relationship of the specimens was obtained through the uniaxial compression test of ordinary concrete and nano-titanium dioxide-modified concrete cube specimens under normal temperature and high-temperature conditions. In addition, the relationship between temperature and damage variables was established, and the unified constitutive model containing damage variables after room temperature and high-temperature treatment of ordinary concrete and nano-titanium dioxide-modified concrete were established. It provides a reference for future research on the mechanical properties of high-performance concrete structures after high temperatures (fire).


Introduction
Under normal room temperature conditions, the general building structure can maintain its intended functionality for an extended period. However, in instances where there exists a substantial temperature differential within the building environment, the structural load-bearing capacity may diminish, leading to a decline in performance and ultimately resulting in structural failure. The incidence of solar radiation on the sun-facing facade during summer months increases the temperature of the exterior surface of the building. However, this temperature generally does not exceed 60 • C, and it will also cause cracks on the surface of the building, affecting the normal use of the building. In addition, some workshops are in a high-temperature environment for a long time, such as some chemical and metallurgical enterprises' high-temperature workshops, and their structural surface temperature can reach 200 • C or higher. When the chimney emits high-temperature gas, the internal temperature can reach 500~600 • C. In some accidental cases, there will be a short-term high-temperature impact on the building, such as the temperature of the building reaching 1000 • C or higher within one hour during a fire. At high temperatures, the pore pressure and porosity of concrete will change, and phenomena such as thermal expansion, thermal cracking, and thermal creep will occur. These phenomena will destroy the mesoscopic structure of concrete, leading to a gradual decline in its mechanical performance and problems such as cracking and spalling on the surface. In addition, concrete can also cause damage due to bending or stiffness and mass loss, etc. Various studies indicate that the main effect of fire (high temperature) on concrete is a change in its properties, leading to spalling, while the stress-strain behavior under high-temperature exposure is complex. Natural and clean river sand was selected and screened with a standard sieve with a pore size of 0.6 mm. The maximum particle size of the test sand is less than 1.2 mm, and most of the particles (more than 99%) are below 900 µm. More than 50% of particles have a particle size of less than 500 µm. The average particle size is 0.46 mm. The gradation curve of river sand is shown in Figure 1.    Limestone crushed stone was used, and the particle size is 5-20 mm continuous grading. The crushed stone used for the crushing index test was passed through a 14 mm test sieve and left on a 10 mm sieve. Put the crushed stone on the sieve into a 100-110 • C oven to dry for four hours, then put it into a cylindrical mold to vibrate and compact, and then put the plunger on top of the aggregate. The integral unit was placed on the pressure testing machine, and the plunger was loaded and gradually pressurized to 400 kN within 10 min. After unloading, the crushed stone was taken out and placed in 2.36 mm for screening, and the ratio of the mass of the crushed stone through this screening to the total mass is the crushing index. The crushing index of the coarse aggregate crushed stone used in the test is 4.8%, and the density is 2.7 g/cm 3 . The grading curve of limestone crushed stone is shown in Figure 2.  The water-reducing agent adopted was 2651F (BASF, Heidelberg, Germany), which is a modified polycarboxylic acid ether made by a spray drying process, which has good fluidity and uniform color.
Nano titanium dioxide (Xfnano, Nanjing, China) is in the form of white powder, as shown in Figure 3, and its physical properties are shown in Table 2. When the aqueous solution was prepared, nano titanium dioxide was found to precipitate in the solution, as shown in Figure 3. The even spreading of nano titanium dioxide in concrete can be achieved by utilizing an appropriate amount of water reducing agent and mechanical mixing, as nano titanium dioxide has been shown to be insoluble in water.

Sample Preparation
The mix ratio is listed in Table 3. According to the results of the previous research, the nano titanium dioxide content of 3% (NTC3 and the notation "NTC3" denotes the incorporation of nano-titanium dioxide into cement at a proportion of 3% of the cement mass) was chosen in this paper [23]. The specific preparation and configuration process of nano-titanium dioxide-modified concrete specimens was referred to the research of Xu et al. [24]. Ordinary concrete was prepared the same way as nano-titanium dioxidemodified concrete without adding titanium dioxide. Concrete samples had cubic specimens with 100 mm inside. The test specimens were created and put through testing in accordance with Standard for Testing Methods for Mechanical Properties of Ordinary Concrete (GB 50081-2002) [25]. The curing period for both types of concrete is 28 days.

Test Equipment
The instrument for the high-temperature treatment of the specimen is a chamber resistance furnace with model SMF1900-50 (Shanghai Haoyue Vacuum Equipment Co., Ltd., Shanghai, China, Figure 4A), and the maximum heating temperature can reach 1900 • C. The test sample heating process is as follows: (1) Fifteen ordinary concrete and fifteen NTC3 specimens were carefully chosen and subsequently partitioned into five distinct groups. (2) After 28 days of natural conservation, it was subjected to high-temperature heat treatment of 200 • C, 400 • C, 600 • C, and 800 • C, respectively. The heating rate in the high-temperature furnace is 5 • C/min. The temperature is constant for 6 h after reaching the target temperature, and then naturally cooled in the furnace for 24 h.
The uniaxial compression testing instrument for concrete specimens is the microcomputercontrolled rigid servo triaxial pressure testing machine produced by Xi'an Lichuang Material Testing Technology Co., Ltd. (Xi'an, China). The maximum load is 2000 kN and the axial load accuracy is ±1%, as shown in Figure 4B. The rate of uniaxial compression test is 0.5 MPa/s. The longitudinal wave velocity test adopts V-METER III ultrasonic pulse velocity tester (James Instruments Inc., Chicago, IL, USA), as shown in Figure 4C, and the test accuracy is 0.1 µs.   Figure 5 shows the apparent characteristics of the concrete specimens after under ing different temperature treatments. After undergoing different temperature treatme there is a clear difference between the apparent characteristics of ordinary concrete a NTC3 specimens. The volume expansion of both was not apparent between 200 °C a 600 °C, and the surface locally changed from gray to brown. From 800 °C, the surface the specimens started to show black spots and volume expansion.

Test Results and Discussion
3.1. Surface Characteristics of Specimens after High Temperature Figure 5 shows the apparent characteristics of the concrete specimens after undergoing different temperature treatments. After undergoing different temperature treatments, there is a clear difference between the apparent characteristics of ordinary concrete and NTC3 specimens. The volume expansion of both was not apparent between 200 • C and 600 • C, and the surface locally changed from gray to brown. From 800 • C, the surface of the specimens started to show black spots and volume expansion.   Figure 5 shows the apparent characteristics of the concrete specimens after undergoing different temperature treatments. After undergoing different temperature treatments, there is a clear difference between the apparent characteristics of ordinary concrete and NTC3 specimens. The volume expansion of both was not apparent between 200 °C and 600 °C, and the surface locally changed from gray to brown. From 800 °C, the surface of the specimens started to show black spots and volume expansion.  Figure 6 shows the compressive stress-strain curve of ordinary concrete after high temperatures. It can be seen that the stress-strain curve of ordinary concrete at room temperature is divided into four stages: the compacting stage, elastic stage, strengthening stage, and unloading stage. After high-temperature treatment, the stress-strain trend of the specimen has a certain change. After 200 °C, the ordinary concrete test specimen reached the stress peak and did not immediately enter the unloading stage, and the residual strain further expanded. As the treatment temperature was elevated, the average peak compressive strength of ordinary concrete exhibited a further decline. Notably, the compressive strength of ordinary concrete experienced a rapid reduction between 400 °C and 800 °C. At 800 °C, the average peak compressive strength of conventional concrete was measured at 23.12 MPa, indicating a decrease of 44.32% in comparison to the initial measurement.

Mechanical Properties of Concrete after High Temperature
In this paper, the slope between the peak stress and 0.1 times the peak stress of the test piece is approximately close to the secant modulus. The approximate secant modulus of ordinary concrete is shown in Table 4. It can be seen that the approximate secant modulus of ordinary concrete is 34.646 GPa. After 200 °C high-temperature treatment, the approximate secant modulus of ordinary concrete is reduced to 20.248 GPa. After 400 °C high-temperature treatment, the approximate secant modulus of ordinary concrete is reduced to 16.7 GPa. As the temperature rises further, the approximate secant modulus of ordinary concrete is further reduced. However, the reduction of 400 °C to 800 °C is not significant, and after 800 °C high-temperature treatment, the approximate secant modulus of ordinary concrete is reduced to 13.072 GPa.  Figure 6 shows the compressive stress-strain curve of ordinary concrete after high temperatures. It can be seen that the stress-strain curve of ordinary concrete at room temperature is divided into four stages: the compacting stage, elastic stage, strengthening stage, and unloading stage. After high-temperature treatment, the stress-strain trend of the specimen has a certain change. After 200 • C, the ordinary concrete test specimen reached the stress peak and did not immediately enter the unloading stage, and the residual strain further expanded. As the treatment temperature was elevated, the average peak compressive strength of ordinary concrete exhibited a further decline. Notably, the compressive strength of ordinary concrete experienced a rapid reduction between 400 • C and 800 • C. At 800 • C, the average peak compressive strength of conventional concrete was measured at 23.12 MPa, indicating a decrease of 44.32% in comparison to the initial measurement.  Figure 6 shows the compressive stress-strain curve of ordinary concrete after high temperatures. It can be seen that the stress-strain curve of ordinary concrete at room temperature is divided into four stages: the compacting stage, elastic stage, strengthening stage, and unloading stage. After high-temperature treatment, the stress-strain trend of the specimen has a certain change. After 200 °C, the ordinary concrete test specimen reached the stress peak and did not immediately enter the unloading stage, and the residual strain further expanded. As the treatment temperature was elevated, the average peak compressive strength of ordinary concrete exhibited a further decline. Notably, the compressive strength of ordinary concrete experienced a rapid reduction between 400 °C and 800 °C. At 800 °C, the average peak compressive strength of conventional concrete was measured at 23.12 MPa, indicating a decrease of 44.32% in comparison to the initial measurement.

Mechanical Properties of Concrete after High Temperature
In this paper, the slope between the peak stress and 0.1 times the peak stress of the test piece is approximately close to the secant modulus. The approximate secant modulus of ordinary concrete is shown in Table 4. It can be seen that the approximate secant modulus of ordinary concrete is 34.646 GPa. After 200 °C high-temperature treatment, the approximate secant modulus of ordinary concrete is reduced to 20.248 GPa. After 400 °C high-temperature treatment, the approximate secant modulus of ordinary concrete is reduced to 16.7 GPa. As the temperature rises further, the approximate secant modulus of ordinary concrete is further reduced. However, the reduction of 400 °C to 800 °C is not significant, and after 800 °C high-temperature treatment, the approximate secant modulus of ordinary concrete is reduced to 13.072 GPa.   In this paper, the slope between the peak stress and 0.1 times the peak stress of the test piece is approximately close to the secant modulus. The approximate secant modulus of ordinary concrete is shown in Table 4. It can be seen that the approximate secant modulus of ordinary concrete is 34.646 GPa. After 200 • C high-temperature treatment, the approximate secant modulus of ordinary concrete is reduced to 20.248 GPa. After 400 • C high-temperature treatment, the approximate secant modulus of ordinary concrete is reduced to 16.7 GPa. As the temperature rises further, the approximate secant modulus of ordinary concrete is further reduced. However, the reduction of 400 • C to 800 • C is not significant, and after 800 • C high-temperature treatment, the approximate secant modulus of ordinary concrete is reduced to 13.072 GPa.  Figure 7 shows the compressive stress-strain curve of NTC3 after high temperature. It can be seen that after high-temperature treatment, the stress-strain trend of the specimen does not change and still presents four stages. At room temperature, the average peak stress of NTC3 was 49.91 MPa. With the further increase of the treatment temperature, the average peak compressive strength of NTC3 is further reduced, similar to ordinary concrete. After 800 • C, the average peak compressive strength of NTC3 is 24.61 MPa, which is 50.69% lower than the initial time. It can be seen that the incorporation of nano-titanium dioxide has an improved effect on the mechanical properties of concrete at temperatures below 600 • C, and it is not helpful to the high-temperature resistance of concrete above 600 • C. Table 5 displays the estimated secant modulus of the specimen based on the calculation method outlined in the preceding section. The approximate secant modulus of nano-titanium dioxide is 31.229 GPa, and after high-temperature treatment at 200 • C, the approximate secant modulus of the specimen is reduced to 22.173 GPa. After hightemperature treatment at 400 • C, the approximate secant modulus of concrete was reduced to 19.46 GPa. As the temperature rises further, the approximate secant modulus of modified concrete further decreases. After high-temperature treatment at 800 • C, the approximate secant modulus of the specimen was reduced to 10.901 GPa.

Mechanical Properties of NTC3 after High Temperature
tion method outlined in the preceding section. The approximate secant modulus of nanotitanium dioxide is 31.229 GPa, and after high-temperature treatment at 200 °C, the approximate secant modulus of the specimen is reduced to 22.173 GPa. After high-temperature treatment at 400 °C, the approximate secant modulus of concrete was reduced to 19.46 GPa. As the temperature rises further, the approximate secant modulus of modified concrete further decreases. After high-temperature treatment at 800 °C, the approximate secant modulus of the specimen was reduced to 10.901 GPa.

Derivation of the Damage Constitutive Equation
Lamaitre [26] proposed the important strain equivalence principle in 1971: in the uniaxial stress state, it is believed that the constitutive equation of the material can derive the constitutive relationship of the damaged material in the absence of damage as long as the stress in it is replaced by the effective stress. Let the total volume of the specimen be V, and the damaged material unit be regarded as various isotropic units. The total volume is composed of two parts, namely the damage zone V d and the undamaged area V n , obtaining: Introducing the damage variable d c , we obtain: Thus, the effective stress σ n and σ can be expressed as where E T is the initial modulus of elasticity after different temperature treatments, and ε is the strain [27]. Tensile and compressive strains mainly induce microcrack extension and elongation in near-brittle materials; therefore, the damage evolution path can be described in strain space. According to plasticity theory, the direction of strain in a material depends on the stress state of the material and not on the direction of the incremental stress in the material. Therefore, the multi-axial stress state can be converted into an equivalent stress state by combining the stress invariants, i.e., the equivalent strain ε eq is where I 1σ is the first invariant of the effective stress tensor; J 2σ is the second invariant of the effective stress tensor; σ max ei is the maximum effective principal stress; · is Macaulaybracket, which can be expressed as x + = (x + |x|)/2 and x + = (x − |x|)/2. where where σ e is the second-order effective stress tensor; tr(.) is a tensor trace operator; C 0 is the fourth-order elastic stiffness tensor of undamaged concrete ( A : B = A ij B ij . First, define the uniform damage loading surface under strain space as: where κ is the damage threshold, which represents the cumulative irreversible damage, i.e., the maximum value of the corresponding local equivalent strain throughout the loading process, and defines it as: Secondly, when the equivalent strain reaches the damage threshold, the concrete begins to suffer, and the initial damage loading surface under the strain space is the ultimate strength surface, which is expressed as: where κ 0 is the initial damage threshold for concrete, defined as: Finally, the initial damage loading surface under the strain space after different temperature treatments is written as: where κ t is the initial damage threshold after different temperature treatments, defined as: where f c is the peak strength of concrete when uniaxial compression; f ctb is the stress corresponding to the inflection point before the stress peak; κ ctb is the damage threshold corresponding to the first inflection point on the stress-strain curve. In the above equation, the strain ε and the damage threshold κ should be satisfied: The damage evolution equation in line with the actual situation was established through the stress-strain curve obtained by the uniaxial compression test of concrete in this paper. Assuming that σ = f (ε) is the constitutive relationship under uniaxial compression of concrete and the stress-strain curve should satisfy: when ε = 0, σ = 0, that is, the curve passes through the coordinate origin. There is only one point on the curve, satisfying dσ/dε = 0, that is, there is only one peak point on the curve, at this time ε = ε t , σ t = f (ε t ). When 0 < ε < ε ctb , d 2 σ/dε 2 > 0, that is, when the stress just begins to increase, the compacting stage of the concrete test block and the slope of the curve increases with the increase of strain. When ε = ε ctb , the curve satisfies d 2 σ/dε 2 = 0, which means this point is the first inflection point on the curve, and it is the turning point of the concrete test block from the elastic stress stage to the elastic-plastic stress stage. When ε ctb < ε < ε t , d 2 σ/dε 2 < 0, before the stress reaches the peak point, the slope of the curve decreases with the increase of strain, and there is no inflection point on this curve. When ε > ε t , there is only one point on the curve that satisfies d 2 σ/dε 2 = 0, which means this curve has only one inflection point. The strain point where the concrete test block is destroyed, and the bearing capacity is lost. Figure 8 depicts the schematic diagram of the constitutive relationship of concrete under uniaxial compression.
Materials 2023, 16, x FOR PEER REVIEW = ( ) . When 0 < < , 2 / 2 > 0 , that is, when the stress just begins crease, the compacting stage of the concrete test block and the slope of the curve inc with the increase of strain. When = , the curve satisfies 2 / 2 = 0, which this point is the first inflection point on the curve, and it is the turning point of the co test block from the elastic stress stage to the elastic-plastic stress stage. When , 2 / 2 < 0, before the stress reaches the peak point, the slope of the curve dec with the increase of strain, and there is no inflection point on this curve. When there is only one point on the curve that satisfies 2 / 2 = 0, which means this has only one inflection point. The strain point where the concrete test block is dest and the bearing capacity is lost. Figure 8 depicts the schematic diagram of the const relationship of concrete under uniaxial compression. According to the above segmentation conditions for the stress-strain curve crete, the stress-strain expression under compression is established. Among them, cending section of the curve is expressed exponentially and rationally, and the desc segment of the curve is expressed in quadratic polynomial and exponential forms bined with the constitutive relationship (4), the evolution equation of compression age dc is derived: According to the above segmentation conditions for the stress-strain curve of concrete, the stress-strain expression under compression is established. Among them, the ascending section of the curve is expressed exponentially and rationally, and the descending segment of the curve is expressed in quadratic polynomial and exponential forms. Combined with the constitutive relationship (4), the evolution equation of compression damage d c is derived: where, γ 1 is the material constant controlling the compaction stage of concrete, which is taken according to the characteristics of the compression-density phase of the stress-strain curve obtained from the uniaxial compression test of concrete in this paper, and the range of values is defined as 2.5-6.0. γ 2 is the material constant controlling the peak strain of concrete, and the range of values is usually 2.0-4.5. Because hightemperature treatment changes the mechanical properties of the material, concrete treated at different temperatures should correspond to different γ 1 and γ 2 . Ψ ctn and Ψ ctd are shape parameters that determine the stress-strain curve, both of which take values in the ranges 0.5-0.9 and 0-0.5, respectively. Where κ ctb and κ ctn are the inflection point damage thresholds before and after reaching the peak stress point, respectively, indicating the strain value corresponding to the inflection point of the compressive stress-strain curve at the softening section.

Damage Constitutive Model of Ordinary Concrete after High Temperature
Figures 9-13 are the stress-strain curves of ordinary concrete after different temperature treatments with the first and second derivatives diagrams of the stress-strain curve. Firstly, the stress-strain curve can obtain the peak strain f c of ordinary concrete after different temperature treatments. Secondly, the initial modulus of elasticity E T after different temperature treatments can be obtained from the stress-strain curve and the first derivative curve of the stress-strain curve. κ t can be obtained by substituting E T into the Equation (15). Finally, the inflection point κ ctn of the stress-strain curve can be obtained from the first derivative curve of the stress-strain curve. The boundary parameters of concrete compression damage d c after different temperature treatments are shown in Tables 6 and 7.

Damage Constitutive Model of Ordinary Concrete after High Temperature
Figures 9-13 are the stress-strain curves of ordinary concrete after different temperature treatments with the first and second derivatives diagrams of the stress-strain curve. Firstly, the stress-strain curve can obtain the peak strain fc of ordinary concrete after different temperature treatments. Secondly, the initial modulus of elasticity ET after different temperature treatments can be obtained from the stress-strain curve and the first derivative curve of the stress-strain curve. κt can be obtained by substituting ET into the Equation (15). Finally, the inflection point κctn of the stress-strain curve can be obtained from the first derivative curve of the stress-strain curve. The boundary parameters of concrete compression damage dc after different temperature treatments are shown in Tables 6 and 7.      . Figure 11. (a) Stress-strain curve of ordinary concrete at 400 °C (b) First derivative of the s strain curve of ordinary concrete at 400 °C (c) Second derivative of the stress-strain curve of ord concrete at 400 °C.       Table 7. Parameters in the descending section of stress-strain curve after different temperature treatment.
Temperature From Equations (5), (15), and (16), combined with the damage evolution parameters in Tables 6 and 7, the constitutive equations of ordinary concrete after different temperature treatments can be obtained as follows: According to Equation (11) and considering the relationship between ε ctb = γ 1 κ ctb , ε t = γ 2 κ t , ε ctn = κ ctn , so that Equation (21) can be written as: Figure 14 compares the theoretical and test curves of the constitutive equation of ordinary concrete after different temperature treatments. It can be seen from the figure that the theoretical curve of ordinary concrete constitutive equation is in good agreement with the test curve, indicating that the damage constitutive model established in this paper can better reflect the stress-strain curve characteristics of concrete uniaxial compression, which has certain practical engineering significance. Figure 14 compares the theoretical and test curves of the constitutive equation of ordinary concrete after different temperature treatments. It can be seen from the figure that the theoretical curve of ordinary concrete constitutive equation is in good agreement with the test curve, indicating that the damage constitutive model established in this paper can better reflect the stress-strain curve characteristics of concrete uniaxial compression, which has certain practical engineering significance.

Damage Constitutive Model of NTC3 after High Temperature
The test curve and the theoretical curve of the constitutive equation for ordinary concrete established in the preceding section correspond very well. The stress-strain test curve for uniaxial compression of nano-modified concrete demonstrates that the trend of the stress-strain curve is consistent with that of ordinary concrete. The peak strength and high-temperature resistance of concrete were improved after adding nanometers. When the temperature ranges from 20 °C to 600 °C, the peak strength of NTC3 increases by 20%. In comparison, when the temperature exceeds 600 °C, the enhancement of the peak strength of the specimen by the addition of TiO2 nanoparticles is not significant. The strengthening coefficient can be defined to reflect the strength increase effect of nano-titanium dioxide on concrete. The strengthening coefficient can be obtained by fitting the peak strength change value of concrete before and after nano addition. The strengthening coefficient is defined as:

Damage Constitutive Model of NTC3 after High Temperature
The test curve and the theoretical curve of the constitutive equation for ordinary concrete established in the preceding section correspond very well. The stress-strain test curve for uniaxial compression of nano-modified concrete demonstrates that the trend of the stress-strain curve is consistent with that of ordinary concrete. The peak strength and high-temperature resistance of concrete were improved after adding nanometers. When the temperature ranges from 20 • C to 600 • C, the peak strength of NTC3 increases by 20%. In comparison, when the temperature exceeds 600 • C, the enhancement of the peak strength of the specimen by the addition of TiO 2 nanoparticles is not significant. The strengthening coefficient can be defined to reflect the strength increase effect of nano-titanium dioxide on concrete. The strengthening coefficient can be obtained by fitting the peak strength change value of concrete before and after nano addition. The strengthening coefficient is defined as: where Q f reflects the strengthening coefficient brought by the addition of nanomaterials to concrete under different temperatures. f n c is the uniaxial compressive strength of NTC3 under different temperatures. f c is the uniaxial compressive strength of ordinary concrete under different temperatures. Table 8 shows the strengthening coefficient Q f of the peak strength of NTC3 compared with ordinary concrete after different temperature treatments. Figure 15 shows the primary, secondary, and cubic polynomial fitting of the strengthening coefficient Q f with respect to the processing temperature. The fitting degree of the quadratic polynomial is good, and the goodness of fit (R 2 ) of the curve is 0.999. Therefore, this relationship can be used to predict the uniaxial compressive strength of NTC3 at different temperatures. The fitting relation is:   Because the uniaxial compressive stress-strain curve of concrete after adding TiO2 nanopowder is consistent with the stress-strain curve trend of ordinary concrete, it only improves at the peak point. Therefore, the strengthening coefficient can be introduced on the basis of the second and third stages of the ordinary concrete constitutive equation established above, and the damage constitutive equation of NTC3 under different temperatures can be obtained. The damage constitutive model of NTC3 after high temperature and the derivation process of the damage evolution equation have been described in the previous section and will not be described here. Figures 16-20 are the first and second derivatives of the stress-strain curve and Because the uniaxial compressive stress-strain curve of concrete after adding TiO 2 nanopowder is consistent with the stress-strain curve trend of ordinary concrete, it only improves at the peak point. Therefore, the strengthening coefficient can be introduced on the basis of the second and third stages of the ordinary concrete constitutive equation established above, and the damage constitutive equation of NTC3 under different temperatures can be obtained. The damage constitutive model of NTC3 after high temperature and the derivation process of the damage evolution equation have been described in the previous section and will not be described here.  are the first and second derivatives of the stress-strain curve and stressstrain curve of NTC3 after different temperature treatments. Firstly, the peak strain f n c of NTC3 after different temperature treatments can be obtained from the stress-strain curve. Secondly, the initial modulus of elasticity can be E T obtained from the stress-strain curve and the first derivative curve of the stress-strain curve. The κ t can be obtained by substituting it into Equation (15). Finally, the inflection point κ ctn of the stress-strain curve can be obtained from the first derivative curve of the stress-strain curve. The boundary parameters of NTC3 compression damage d c after different temperature treatments are shown in Tables 9 and 10.
Secondly, the damage constitutive equation of NTC3 under different temperatures can be obtained by substituting (25) into Equation (5). Figure 21 compares the theoretical and test curves of the constitutive equation of NTC3 after different temperature treatments. From the figure, the theoretical curve of NTC3 constitutive equation is in good agreement with the experimental curve, indicating that the NTC3 damage constitutive model established in this paper can better reflect the stress-strain curve characteristics of NTC3 uniaxial compression, which verifies the rationality and reliability of the model and the model parameter determination method, which has certain practical significance.
Secondly, the damage constitutive equation of NTC3 under different temperature can be obtained by substituting (25) into Equation (5).

Conclusions
In this paper, the mechanical properties of ordinary concrete and NTC3 after high temperature are analyzed and compared, mainly through experimental and theoretica analysis, and the damage constitutive model of ordinary concrete and NTC3 is estab lished.
(1) Ordinary concrete and NTC3 specimens were subjected to various temperature ranging from 20 °C to 800 °C. Notably, the volume expansion of both materials was not apparent within the temperature range of 200 °C to 600 °C. Additionally, the sur face color of the specimens transitioned from gray to brown. At a temperature of 800

Conclusions
In this paper, the mechanical properties of ordinary concrete and NTC3 after high temperature are analyzed and compared, mainly through experimental and theoretical analysis, and the damage constitutive model of ordinary concrete and NTC3 is established.
(1) Ordinary concrete and NTC3 specimens were subjected to various temperatures ranging from 20 • C to 800 • C. Notably, the volume expansion of both materials was not apparent within the temperature range of 200 • C to 600 • C. Additionally, the surface color of the specimens transitioned from gray to brown. At a temperature of 800 • C, the specimen exhibits the formation of black spots on its surface and undergoes volumetric expansion. (2) With the increase of temperature, ordinary concrete's average peak compressive resistance is further reduced. At 800 • C, the average peak compressive strength of ordinary concrete was 23.120 MPa, which decreased by 44.32% compared with the initial time, and the approximate secant modulus decreased to 13.072 GPa. Similar to ordinary concrete, after high-temperature treatment from 400 • C to 800 • C, the compressive strength of NTC3 decreased, and the average peak compressive strength of NTC3 was 24.610 MPa at 800 • C, a decrease of 50.69% compared with the initial time. It can be seen that the incorporation of nano titanium dioxide at lower than 600 • C can help the high-temperature resistance of concrete, and when it is higher than 600 • C, the mechanical properties of ordinary concrete and NTC3 compression are basically no different. (3) The stress-strain curves exhibited by ordinary concrete specimens subjected to uniaxial compression and titanium nanoconcrete specimens prior to and subsequent to high-temperature exposure exhibit similar shapes and characteristics. A constitutive relationship formula was established for the stress-strain curve of ordinary concrete specimens and NTC3 under uniaxial compression. A constitutive relationship for the uniaxial compressive stress-strain behavior of concrete was established, taking into account the variable of high-temperature damage. The constitutive relationship of concrete under high temperatures has been enhanced in accordance with the law of continuous change. Funding: This research was funded by "Natural Science Foundation Project of Shanghai Science and Technology Commission", grant number 23ZR1443600.